High-mobility three-atom-thick semiconducting films with wafer-scale homogeneity Kibum Kang1*, Saien Xie2*, Lujie Huang1, Yimo Han2, Pinshane Y. Huang2, Kin Fai Mak3,4, Cheol-Joo Kim1, David Muller2,3 & Jiwoong Park1,3
The large-scale growth of semiconducting thin films forms the basis of modern electronics and optoelectronics. A decrease in film thickness to the ultimate limit of the atomic, sub-nanometre length scale, a difficult limit for traditional semiconductors (such as Si and GaAs), would bring wide benefits for applications in ultrathin and flexible electronics, photovoltaics and display technology1–3. For this, transition-metal dichalcogenides (TMDs), which can form stable three-atom-thick monolayers4, provide ideal semiconducting materials with high electrical carrier mobility5–10, and their largescale growth on insulating substrates would enable the batch fabrication of atomically thin high-performance transistors and photodetectors on a technologically relevant scale without film transfer. In addition, their unique electronic band structures provide novel ways of enhancing the functionalities of such devices, including the large excitonic effect11, bandgap modulation12, indirect-todirect bandgap transition13, piezoelectricity14 and valleytronics15. However, the large-scale growth of monolayer TMD films with spatial homogeneity and high electrical performance remains an unsolved challenge. Here we report the preparation of high-mobility 4-inch wafer-scale films of monolayer molybdenum disulphide (MoS2) and tungsten disulphide, grown directly on insulating SiO2 substrates, with excellent spatial homogeneity over the entire films. They are grown with a newly developed, metal–organic chemical vapour deposition technique, and show high electrical performance, including an electron mobility of 30 cm2 V21 s21 at room temperature and 114 cm2 V21 s21 at 90 K for MoS2, with little dependence on position or channel length. With the use of these films we successfully demonstrate the wafer-scale batch fabrication of highperformance monolayer MoS2 field-effect transistors with a 99% device yield and the multi-level fabrication of vertically stacked transistor devices for three-dimensional circuitry. Our work is a step towards the realization of atomically thin integrated circuitry. Existing growth methods for large-scale monolayer TMDs have so far produced materials with limited spatial uniformity and electrical performance. For instance, the sulphurization of metal or metal compounds only provides control over the average layer number, producing spatially inhomogeneous mixtures of monolayer, multi-layer and no-growth regions16,17. Although chemical vapour deposition (CVD) based on solid-phase precursors (such as MoO3, MoCl5 or WO3)18–23 has shown better thickness control on a large scale, the electrical performance of the resulting material, which is often reported from a small number of devices in selected areas, fails to show spatially uniform high carrier mobility. Here we report the growth of semiconducting monolayer films of MoS2 and tungsten disulphide (WS2) on silicon oxide on a 4-inch wafer scale, with both excellent electrical performance and structural continuity, maintained uniformly over the entire films. Figure 1 presents our continuous TMD monolayer films and shows their waferscale homogeneity and intrinsic optical properties. The colour photos of MoS2 (Fig. 1a; greenish yellow) and WS2 (Fig. 1b; yellow) films
grown on a transparent 4-inch fused silica wafer show that the TMD grown region (right half) is uniform over the whole substrate and clearly distinguishable from the bare silica substrate (left half). The optical absorption, photoluminescence and Raman spectra measured from our films show characteristics unique to monolayer MoS2 and WS2, respectively (Fig. 1d–f). All of these measured spectra have the same peak positions as in exfoliated monolayer samples (denoted by diamonds)13,24–26, regardless of the location of the measurements within our films (Supplementary Fig. 1). The X-ray photoelectron spectra taken from our monolayer MoS2 film show almost identical features to those of bulk single crystal with a low level of defects, further confirming the precise chemical composition and the high quality of our MoS2 film (Supplementary Fig. 2). Figure 1c shows a photo of a MoS2 film grown on a 4-inch SiO2/Si wafer. The monolayer film was patterned using standard photolithography and oxygen plasma etching to form MoS2-covered squares (dark, 6 mm wide) with an array of 3 mm holes. An enlarged, normalized optical reflection image (Fig. 1h) displays a homogeneous reflection contrast for the entire MoS2-covered region, confirming uniform monolayer growth everywhere with no gaps. In addition, Fig. 1g shows a scanning electron microscope (SEM) image of an array of fully suspended monolayer MoS2 membranes (2 mm in diameter) fabricated by transferring our metal–organic chemical vapour deposition (MOCVD)-grown film onto a SiN grid with holes. Its high fabrication yield (.99.5%) suggests mechanical strength and continuity of the film. The widefield photoluminescence images of these films (insets to Fig. 1g, h) show strong, spatially uniform photoluminescence signals, further confirming that they are continuous monolayer MoS2, with its high quality maintained even after patterning or transfer. The same spatial uniformity was seen in the optical reflection and photoluminescence images of a monolayer WS2 film that was similarly grown and patterned (Fig. 1i). Together, the data in Fig. 1 confirm that our MoS2 and WS2 films are continuous monolayers, spatially uniform over the entire 4-inch growth substrates with intrinsic optical properties. Below, using MoS2 as the main example, we discuss the growth (Fig. 2) and the excellent electrical properties (Fig. 3) of these MOCVD-grown films. Figure 2a schematically explains our MOCVD growth, where we only use gas-phase precursors of Mo(CO)6, W(CO)6, (C2H5)2S and H2, all diluted in argon as a carrier gas (see Supplementary Methods). The concentration of each reactant can be precisely controlled during the entire growth time by regulating the partial pressure (PX) of each reactant X. Thus our setup offers an ideal environment for maximizing the areal coverage of the monolayer and for engineering the film structure by controlling the nucleation density and intergrain stitching. Figure 2 summarizes our key findings. First, our MoS2 film is grown in the layer-by-layer growth mode, which is ideal for uniform layer control over the large scale. Figure 2c plots the areal coverage of monolayer (h1L) and multilayer (h$2L; mostly bilayer) regions measured from our MoS2 grown on SiO2/Si;
Department of Chemistry and Chemical Biology, Cornell University, Ithaca, New York 14853, USA. 2School of Applied and Engineering Physics, Cornell University, Ithaca, New York 14853, USA. 3Kavli Institute at Cornell for Nanoscale Science, Ithaca, New York 14853, USA. 4Laboratory of Atomic and Solid State Physics, Cornell University, Ithaca, New York 14853, USA. *These authors contributed equally to this work. 6 5 6 | N AT U R E | VO L 5 2 0 | 3 0 A P R I L 2 0 1 5 G2015
Macmillan Publishers Limited. All rights reserved
LETTER RESEARCH S
a 4 inches
ML MoS2 Hole SiN
ML MoS2 PL
1.8 2.1 2.4
350 400 450 1.8 1.9 2.0 2.1
Raman shift (cm–1)
ML WS2 PL at 1.9 eV
PL at 2.0 eV
Figure 1 | Wafer-scale monolayer TMD films. a, b, Photographs of monolayer MoS2 (a) and WS2 (b) films grown on 4-inch fused silica substrates, with diagrams of their respective atomic structures. The left halves show the bare fused silica substrate for comparison. c, Photograph of patterned monolayer MoS2 film on a 4-inch SiO2/Si wafer (the darker areas are covered by MoS2). d, Optical absorption spectra of MOCVD-grown monolayer MoS2 (red line) and WS2 (orange line) films in the photon energy range from 1.6 to 2.7 eV. e, Raman spectra of as-grown monolayer MoS2 and WS2, normalized to the silicon peak intensity. f, Normalized photoluminescence spectra of
as-grown monolayer MoS2 and WS2. The peak positions in d–f are consistent with those seen from exfoliated samples (diamonds). g, SEM image and photoluminescence (PL) image (bottom inset, at 1.9 eV) of monolayer (ML) MoS2 membranes suspended over a SiN TEM grid with 2 mm holes (a diagram of the suspended film is shown in the top inset). Scale bar, 10 mm. h, i, Optical images (normalized to the bare substrate region) of patterned monolayer MoS2 (h) and WS2 (i) on SiO2, taken from the wafer-scale patterned films. The insets show photoluminescence images at 1.9 eV (h) and 2.0 eV (i). Scale bars, 10 mm.
Fig. 2b shows optical images at different growth times, revealing the initial nucleation on the SiO2 surface (t 5 0.5t0), subsequent monolayer growth near (0.8t0) and at the maximum monolayer coverage (t0), followed by nucleation mainly at grain boundaries (1.2t0) and bilayer growth (2t0). We observed no nucleation of a second layer while the first layer was forming (h$2L < 0 when t , t0), producing an optimal growth time t0 near full monolayer coverage (h1L < 1). Additional photoluminescence and electron microscope images taken after different growth times further suggested that the edge attachment was the main mechanism for the monolayer growth after nucleation and that the neighbouring monolayer grains were uniformly connected by tilt grain boundaries with enhanced photoluminescence19 at t 5 t0 (see Supplementary Notes and Supplementary Figs 3 and 4). The standard thin-film growth model27 suggests that this growth mode is effective below a certain deposition rate of the growth species, above which it suggests a different mode that forms thicker islands. Indeed, the layer-by-layer growth of MoS2 film was observed only when we applied a low partial pressure (PMo < 1024 Torr in Fig. 2b, c) of Mo vapour (produced by the thermal decomposition of Mo(CO)6; see Supplementary Notes and Supplementary Fig. 5) in the presence of excess (C2H5)2S. In contrast, the growth at a higher PMo was no longer in the layer-by-layer growth mode, instead simultaneously producing a mixture of monolayer, multilayer and no-growth regions (Supplementary Fig. 6). For the uniform monolayer growth over a large substrate, it is thus important to maintain a low PMo constantly over the entire growth region and over time, the key technical capability provided by our MOCVD setup (see Supplementary Fig. 7 for the spatially homogeneous monolayer nucleation on a multi-inch scale). Second, the grain structure of our MoS2 film, including the average grain size and the intergrain connection, depends sensitively on the concentrations of H2, (C2H5)2S as well as residual water. As a representative example, Fig. 2d shows the two main effects of H2, whose presence is necessary for removing carbonaceous species generated during the MOCVD growth: the average grain size increases from hundreds of nanometres to more than 10 mm with decreasing H2 flow, and the MoS2 grains grown under higher H2 flow (Fig. 2d, right image)
have mostly perfect triangular shapes without merging with neighbouring grains, a trend that disappears with lower H2 flow (left and middle images). These observations are consistent with the H2-induced decomposition of (C2H5)2S (increasing nucleation due to hydrogenolysis)28 and the etching of the MoS2 (preventing intergrain connection)29 as reported previously. (For further discussion on the effects of (C2H5)2S and water, see Supplementary Notes and Supplementary Fig. 6.) To grow continuous monolayer MoS2 with a large grain size and highquality intergrain stitching, we thus flowed optimal amounts of H2 and (C2H5)2S and dehydrated the growth environment. The darkfield transmission electron microscope (DF-TEM) and annular darkfield scanning TEM (ADF-STEM) images shown in Fig. 2e, f confirm the structural continuity of our MoS2 film grown under those conditions on the nanometre and atomic length scales. The DF-TEM image shows a continuous polycrystalline monolayer film with no visible gaps and a bilayer area of less than 0.5%. Further analysis of the DF-TEM and electron diffraction data (see Supplementary Fig. 8) confirms a uniform angular distribution of crystal orientations with no preferred intergrain tilt angle for grain boundaries. The ADF-STEM data (Fig. 2f; more images are shown in Supplementary Fig. 9) further confirm that adjacent grains are likely to be connected by a high-quality lateral connection with structures similar to those seen in previous reports18,19. The MoS2 films shown in Fig. 1 as well as those whose electrical properties we show in Figs 3 and 4 were grown under the conditions described in Supplementary Methods, producing an average grain size of ,1 mm (see Fig. 2b, e). Almost identical growth parameters with PW < 1024 Torr produced monolayer WS2 films as shown in Fig. 1b, i, indicating the same layerby-layer growth for WS2 with a similar t0. The electrical properties of our monolayer MoS2 films have two important characteristics: the spatial uniformity over a large scale and excellent transport properties similar to those seen in exfoliated samples. All our electrical measurements in Figs 3 and 4 (except those in Fig. 3c) were performed at room temperature. Figure 3a shows a plot of sheet conductance (s%) against backgate voltage (VBG) measured from a monolayer MoS2 field-effect transistor (FET; optical image 3 0 A P R I L 2 0 1 5 | VO L 5 2 0 | N AT U R E | 6 5 7
Macmillan Publishers Limited. All rights reserved
RESEARCH LETTER a
MFC (C2H5)2S Mo(CO)6 W(CO)6 H2 and Ar 0.5 t0
1.0 0.8 θ1L
0.4 0.2 0 0
1.0 Growth time (t/t0)
Increasing H2 flow
Grain boundary S Mo
Figure 2 | MOCVD growth of continuous monolayer MoS2 film. a, Diagram of our MOCVD growth setup. Precursors were introduced to the growth setup with individual mass flow controllers (MFCs). Red, Mo or W atom; yellow, S atom; white, carbonyl or ethyl ligand. b, Optical images of MOCVD-grown MoS2 at the indicated growth times, where t0 was the optimal growth time for full monolayer coverage. Scale bar, 10 mm. c, Coverage ratio for monolayer (h1L, green) and multi-layer (h$2L, purple) regions as a function of growth time. d, Grain size variation of monolayer MoS2 depending on the hydrogen flow rate; from left to right, 5 standard cm3 min21 (sccm) (SEM image shown), 20 sccm (SEM) and 200 sccm (TEM). e, False-colour DF-TEM image showing a continuous monolayer MoS2 film. Scale bar, 1 mm. f, ADF-STEM image of a laterally stitched grain boundary in a monolayer MoS2 film, with red and yellow dots representing the Mo and S atoms, respectively. Scale bar, 1 nm.
shown in the inset) with multiple electrodes for the four-probe measurements (except for a channel length L of 34 mm). It includes several curves for different L ranging between 1.6 and 34 mm (shifted from the bottom curve for clarity), all of which show nearly identical behaviours, including the n-type conductance, carrier concentration (,4 3 1012 cm22 at VBG 5 0 V) and high field-effect mobility (mFE). Figure 3b further plots mFE measured from five such devices, fabricated at random locations and separated by up to 3.3 mm on a single chip. All the devices show similar mFE near 30 cm2 V21 s21, independent of L and device location, with similarly uniform s%–VBG curves (shown in Supplementary Fig. 10), suggesting the spatial homogeneity of the
electrical properties of the MoS2 film at length scales ranging from micrometres to millimetres. The distribution of mFE of our devices is compared with the results of multiple devices from two previous reports, each measured from individual grains of exfoliated7 or CVD-grown21 MoS2 samples. We find that mFE measured from our MOCVD film is similar to the median mFE (denoted by a star) of exfoliated samples (and several times higher than the CVD results) and has a much narrower distribution. In addition, the temperature dependence of mFE (Fig. 3c) measured from the same device in Fig. 3a shows higher mFE at lower temperatures (92 cm2 V21 s21 at 100 K) and intrinsic, phonon-limited electron transport similar to the behaviours previously observed in exfoliated samples (data from ref. 6 shown in Fig. 3c) but different from those observed from a CVD sample with stronger effects from defects30. Specifically, our data show that the temperature dependence of mobility follows a power law of mFE < T2c with exponent c 5 1.6 for temperatures between 150 and 300 K, close to the value (1.69) predicted by theory5 and consistent with results from previous experiments (average value ranging between 0.6 and 1.7)6–9 for a similar temperature range. Finally, Fig. 3d shows a high-performance MoS2 FET fabricated with an individual top-gate electrode (VTG). It has a high on/off conductance ratio (,106), current saturation at relatively low bias VSD (lower inset to Fig. 3d), high field-effect mobility (,29 cm2 V21 s21) and large transconductance (,2 mS mm21), all of which are comparable to the best reported results6–8. We note that our devices studied in Fig. 3a–d were fabricated at random locations using a polycrystalline monolayer MoS2 film, unlike the devices with singlegrain samples used for comparison. In addition, the electrical properties measured from a separate monolayer MoS2 film with a larger average grain size of 3 mm (instead of 1 mm in Fig. 3) have almost identical characteristics, including the channel-length independence of mFE and the phonon-limited transport at T . 150 K (see Supplementary Fig. 11; with the low-temperature mobility as high as 114 cm2 V21 s21 at 90 K). Taken together, our data confirm the spatial uniformity and high electrical performance of our MoS2 FETs independent of the average grain size, which suggests that the intergrain boundaries in our film do not significantly degrade their electrical transport properties. This is probably due to the formation of well-stitched intergrain boundaries with a low level of defects, an explanation also supported by the ADF-STEM (Fig. 2f) and X-ray photoelectron spectrum data (Supplementary Fig. 2) discussed above. Our data therefore lead us to conclude that our optimized MOCVD growth provides an electrically homogeneous monolayer MoS2 film. Moreover, we successfully fabricated and measured 60 FETs by using a monolayer WS2 film. Even though the growth of monolayer WS2 was not carefully optimized, these devices showed excellent electrical properties, with their mFE as high as 18 cm2 V21 s21 at room temperature (Fig. 3e) and a median mFE close to 5 cm2 V21 s21. In addition, the WS2 device in Fig. 3e showed a high on/off ratio of 106 and the current saturation behaviour (inset to Fig. 3e) as in our MoS2 devices. (See Supplementary Fig. 12 for data from additional monolayer WS2 FET devices). The structural and electrical uniformity of our MoS2 film enables the wafer-scale batch fabrication of high performance FETs as demonstrated in Fig. 3f, g. Figure 3f shows a photo of 8,100 MoS2 FETs with a global back gate, which were fabricated on a 4-inch SiO2/Si wafer with a standard photolithography process. The middle and bottom insets to Figure 3f show colour-scale maps of s% measured from 100 MoS2 FETs in one square region at VBG 5 150 V and 250 V, respectively; the top inset to Fig. 3f shows an enlarged optical image of the devices. We observed an almost perfect device yield of 99%; only two out of 200 FETs that we characterized (including data from an adjacent region) did not conduct. Our data also confirm the spatially uniform n-type transistor operation (larger s% for positive VBG) with similar VBG dependence for all our devices and high on-state device conductance. We further observed similarly uniform VBG dependence from FET devices fabricated using monolayer MoS2 films with different average grain sizes, as characterized by the histograms of the threshold voltages
6 5 8 | N AT U R E | VO L 5 2 0 | 3 0 A P R I L 2 0 1 5 G2015
Macmillan Publishers Limited. All rights reserved
20 L = 1.6 μm
50 γ = 1.7
1.6 2.6 4.6 8.6 34 L (μm)
2.0 V 1.5 VVTG 1.0 V 0.0 V
γ = 1.6
μ FE (cm2 V–1 s–1)
μ FE (cm2 V–1 s–1)
200 T (K)
1 VSD (V)
2.0 V 1.5 V VTG 1.0 V 0.0 V
VBG = 50 V
VBG = –50 V
–8 –6 log( σ /S)
Figure 3 | Electrical characterization and batch fabrication of monolayer TMD FETs. a, Gate-dependent sheet conductance (s%) of monolayer MoS2 FETs measured at different channel lengths L (curves displaced from the bottom for clarity). Inset: optical image of the device; scale bar, 10 mm. b, Fieldeffect mobility (mFE) measured from five MoS2 FETs (ellipses) fabricated at random locations with different L. Data from previous results for CVD-grown samples21 (squares) and exfoliated samples7 (triangles) are shown for comparison (purple stars indicate their medians). c, Temperature dependence of mFE measured from the device in Fig. 3a at L 5 1.6 mm (orange) and 8.6 mm (red), and from a previous report on exfoliated samples6 (grey), both showing phonon-limited intrinsic transport. d, Top gate (VTG)-dependent s% for dual-gate monolayer MoS2 FET (device shown in the upper inset). Lower inset:
VTG-dependent ISD–VSD curves showing current saturation and ohmic electrode contact. Scale bar, 10 mm. e, Gate-dependent s% of a monolayer WS2 FET showing mFE 5 18 cm2 V21 s21. Inset: VTG-dependent ISD–VSD curves showing current saturation and ohmic electrode contact. f, Batch-fabricated 8,100 MoS2 FET devices on a 4-inch SiO2/Si wafer. Top inset: enlarged image of one square containing 100 devices. Middle and bottom insets: corresponding colour maps of s% at gate bias VBG 5 50 V and 250 V, respectively, with the black block in the middle inset representing the only non-conducting device. g, Histogram of on-state and off-state s% of 100 dual-gate FETs showing a median on–off ratio of 106 and a high on-state conductivity. Dark blue, VTG 5 25 V; pale blue, VTG 5 15 V. All measurements were performed at room temperatures except those in c.
(Supplementary Fig. 13). Similarly, we fabricated 100 individually addressable dual-gate MoS2 FETs (similar to the device in Fig. 3d) on another wafer piece. The histogram of the on-state s% (VTG 5 5 V; median carrier concentration ,7 3 1012 cm22) and off-state s% (VTG 5 -5 V) collected from all such FETs (Fig. 3g) shows strong peaks above 1025 S and near 10211 S, respectively, confirming a uniform conductance switching behaviour with high on-state s% (.10 mS) and on–off ratio (,106). In addition, most of these batch-fabricated FETs had a high mFE (.10 cm2 V21 s21; see Supplementary Fig. 14). The data presented in Figs 1–3 confirm the structural and electrical uniformity of the wafer-scale monolayer MoS2 film grown by our MOCVD method. This makes our film compatible with batch device fabrication processes on a technologically relevant scale. Moreover, because SiO2 provides a substrate for its growth, one can produce high-quality monolayer films on a variety of substrates by depositing SiO2 before the growth. This versatility would permit the fabrication of high-performance FETs directly on non-conventional substrates, such as metal and thermally stable plastic. In addition, one can integrate multiple layers of MoS2 devices by repeating the TMD film growth, device fabrication and SiO2 deposition, which could enable novel three-dimensional circuitry. In Fig. 4 we demonstrate this unique potential by producing multi-stacked monolayer MoS2 films as well as electronic devices fabricated at different vertical levels. Figure 4a shows diagrams and photographs of three substrates each with single, double or triple monolayer MoS2 films grown at different levels. The first (bottom) monolayer film was grown on a fused silica substrate; the additional layers were grown on SiO2 (100 nm thick) deposited on the previously grown MoS2 monolayer by using plasma-enhanced CVD. The colour of the substrate, which remains uniform for each substrate, becomes darker as the number of layers increases. Their absorption spectra, shown in Fig. 4b, present almost identical absorption at all
measured wavelengths, once normalized by the number of stacks grown (see the inset), suggesting little degradation of the optical properties of the monolayer MoS2 films after subsequent oxide deposition and MoS2 growth. Figure 4c shows successive diagrams of our multi-stacked device fabrication process: growth of the first MoS2 monolayer on a SiO2/ Si wafer, FET fabrication, deposition of SiO2 (thickness 500 nm; see Supplementary Methods for details), and growth of the second MoS2 monolayer and FET fabrication. A false-colour SEM image in Fig. 4d shows an array of MoS2 FETs successfully fabricated with this process. It includes functioning MoS2 FETs located at two different vertical levels whose conductance can be simultaneously modulated with a global back gate. The ISD–VSD curves measured from two FETs, adjacent both laterally and vertically (see the inset to Fig. 4d), are shown in Fig. 4e. Both devices show a VBG-dependent conductance change (notice the smaller change for the second layer) with an on-state s% of 2.5 mS (first layer) and 1.5 mS (second layer), respectively. Furthermore, we measured similar mFE values (11.5 and 8.8 cm2 V21 s21) from the two devices (Supplementary Fig. 15). The two monolayer MoS2 films were grown on SiO2 substrates prepared differently, and the first-layer device had gone through additional steps, including the second MoS2 growth. Our data in Fig. 4 thus confirm the compatibility of our MOCVD-grown MoS2 films with conventional thin-film deposition and multistacking, which could be used to develop a three-dimensional device architecture based on TMD. Our high-mobility monolayer TMD films can be used immediately for the batch fabrication of TMD-based integrated circuitry consisting of FETs, photodetectors and light emitting diodes, on a technologically relevant multi-inch wafer scale. In addition, because our MOCVD growth is controlled by the kinetics of precursor supply rather than specific precursor–substrate chemistry 3 0 A P R I L 2 0 1 5 | VO L 5 2 0 | N AT U R E | 6 5 9
Macmillan Publishers Limited. All rights reserved
RESEARCH LETTER Triple
Triple/3 Double/2 Single
7. 8. 9.
10. Fused silica
500 600 700 Wavelength (nm)
12. 13. 14.
Figure 4 | Multi-stacking of MoS2/SiO2 structure. a, Diagrams (left) and optical images (right) of single, double and triple stacking of monolayer MoS2/SiO2. b, Optical absorption spectra for single, double and triple stacks, respectively (normalized spectra shown in the inset). c, Diagram for fabrication of MoS2 device/SiO2 stacking by alternating MOCVD growth, device fabrication with photolithography, and SiO2 deposition. See the text for details. d, False-colour SEM image of MoS2 FET arrays on first (bottom) and second (top) layers (the inset shows an enlarged image of a pair of devices in the same relative positions as in the main panel; scale bar, 50 mm). e, ISD–VSD curves measured from two neighbouring devices on the first (left) and second (right) layers, both showing n-type conductance switching. For the first layer, VBG 5 50 V (green) and 250 V (grey); for the second layer, VBG 5 100 V (yellow) and 2100 V (grey).
19. 20. 21. 22. 23. 24. 25. 26. 27.
(an example of the latter would be the different graphene growth modes on copper and nickel), its use is not limited to the TMD– substrate combinations reported here. Instead, it could be generalized for producing various TMD materials, both semiconductor (for example MoSe2 or WTe2) and metal (for example NbSe2 or TaS2), with precise layer control over a large scale. Indeed, our data show that, as an initial demonstration, monolayer TMD growth is possible on a variety of other technologically important substrates (such as Al2O3, SiN and HfO2) with the same growth conditions as those developed for SiO2 (see Supplementary Fig. 16 for MoS2 growth and device fabrication on these substrates, using these nonoptimized conditions). Our versatile MOCVD growth therefore provides a new avenue for the growth, patterning and integration of multiple high-quality monolayer TMD films with different compositions and electrical properties on a single substrate, enabling the future development of atomically thin integrated circuitry. Received 25 November 2014; accepted 13 March 2015. 1. 2. 3. 4.
Rogers, J. A., Someya, T. & Huang, Y. Materials and mechanics for stretchable electronics. Science 327, 1603–1607 (2010). Ko, H. et al. Ultrathin compound semiconductor on insulator layers for highperformance nanoscale transistors. Nature 468, 286–289 (2010). Mitzi, D. B., Kosbar, L. L., Murray, C. E., Copel, M. & Afzali, A. High-mobility ultrathin semiconducting films prepared by spin coating. Nature 428, 299–303 (2003). Geim, A. K. & Grigorieva, I. V. Van der Waals heterostructures. Nature 499, 419–425 (2013).
28. 29. 30.
Kaasbjerg, K., Thygesen, K. S. & Jacobsen, K. W. Phonon-limited mobility in n-type single-layer MoS2 from first principles. Phys. Rev. B 85, 115317 (2012). Baugher, B. W. H., Churchill, H. O. H., Yang, Y. & Jarillo-Herrero, P. Intrinsic electronic transport properties of high-quality monolayer and bilayer MoS2. Nano Lett. 13, 4212–4216 (2013). Radisavljevic, B. & Kis, A. Mobility engineering and a metal–insulator transition in monolayer MoS2. Nature Mater. 12, 815–820 (2013). Schmidt, H. et al. Transport properties of monolayer MoS2 grown by chemical vapor deposition. Nano Lett. 14, 1909–1913 (2014). Jariwala, D. et al. Band-like transport in high mobility unencapsulated single-layer MoS2 transistors. Appl. Phys. Lett. 102, 173107 (2013). Ovchinnikov, D. et al. Electrical transport properties of single-layer WS2. ACS Nano 8, 8174–8181 (2014). Ye, Z. et al. Probing excitonic dark states in single-layer tungsten disulphide. Nature 513, 214–218 (2014). Feng, Q. et al. Growth of large-area 2D MoS2(12x)Se2x semiconductor alloys. Adv. Mater. 26, 2648–2653 (2014). Mak, K. F., Lee, C., Hone, J., Shan, J. & Heinz, T. F. Atomically thin MoS2: a new directgap semiconductor. Phys. Rev. Lett. 105, 136805 (2010). Wu, W. et al. Piezoelectricity of single-atomic-layer MoS2 for energy conversion and piezotronics. Nature 514, 470–474 (2014). Mak, K. F., McGill, K. L., Park, J. & McEuen, P. L. The valley Hall effect in MoS2 transistors. Science 344, 1489–1492 (2014). Lin, Y.-C. et al. Wafer-scale MoS2 thin layers prepared by MoO3 sulfurization. Nanoscale 4, 6637–6641 (2012). Song, I. et al. Patternable large-scale molybdenium disulfide atomic layers grown by gold-assisted chemical vapor deposition. Angew. Chem. Int. Ed. 53, 1266–1269 (2014). Najmaei, S. et al. Vapour phase growth and grain boundary structure of molybdenum disulphide atomic layers. Nature Mater. 12, 754–759 (2013). Van der Zande, A. M. et al. Grains and grain boundaries in highly crystalline monolayer molybdenum disulphide. Nature Mater. 12, 554–561 (2013). Lee, Y.-H. et al. Synthesis and transfer of single-layer transition metal disulfides on diverse surfaces. Nano Lett. 13, 1852–1857 (2013). Liu, H. et al. Statistical study of deep submicron dual-gated field-effect transistors on monolayer chemical vapor deposition molybdenum disulfide films. Nano Lett. 13, 2640–2646 (2013). Yu, Y. et al. Controlled scalable synthesis of uniform, high-quality monolayer and few-layer MoS2 films. Sci. Rep. 3, 1866 (2013). Zhang, Y. et al. Controlled growth of high-quality monolayer WS2 layers on sapphire. ACS Nano 7, 8963–8971 (2013). Zhao, W. et al. Evolution of electronic structure in atomically thin sheets of WS2 and WSe2. ACS Nano 7, 791–797 (2013). Li, H. et al. From bulk to monolayer MoS2: evolution of Raman scattering. Adv. Funct. Mater. 22, 1385–1390 (2012). Berkdemir, A. et al. Identification of individual and few layers of WS2 using Raman spectroscopy. Sci. Rep. 3, 1755 (2013). King, D. A. & Woodruff, D. P. Growth and Properties of Ultrathin Epitaxial Layers (Elsevier, 1997). Connor, R. & Adkins, H. Hydrogenolysis of oxygenated organic compounds. J. Am. Chem. Soc. 54, 4678–4690 (1932). Cristol, S. et al. Theoretical study of the MoS2 (100) surface: a chemical potential analysis of sulfur and hydrogen coverage. J. Phys. Chem. B 104, 11220–11229 (2000). Najmaei, S. et al. Electrical transport properties of polycrystalline monolayer molybdenum disulfide. ACS Nano 8, 7930–7937 (2014).
Supplementary Information is available in the online version of the paper. Acknowledgements We thank P. L. McEuen, M.-H. Jo, H. Heo and H.-C. Choi for discussions, and M. Guimaraes and Z. Ziegler for help in preparing the manuscript. This work was supported mainly by the AFOSR (FA2386-13-1-4118 and FA9550-11-1-0033) and the Nano Material Technology Development Program through the National Research Foundation of Korea (NRF) funded by the Ministry of Science, ICT, and Future Planning (2012M3A7B4049887). Additional funding was provided by the National Science Foundation (NSF) through the Cornell Center for Materials Research (NSF DMR-1120296) and by the Samsung Advanced Institute for Technology GRO Program. Device fabrication was performed at the Cornell NanoScale Facility, a member of the National Nanotechnology Infrastructure Network, which is supported by the National Science Foundation (ECS-0335765). Author Contributions K.K. and S.X. contributed equally to this work. K.K, S.X. and J.P. conceived the experiments. K.K. and S.X. performed the synthesis, optical characterization, device fabrication, and electrical measurements. L.H. conducted low-temperature electrical measurement, with assistance from K.F.M. Y.H, P.Y.H. and D.A.M. performed atomic resolution STEM imaging. K.K. carried out DF-TEM and data analysis, with assistance from C.-J.K. K.K, S.X. and J.P. wrote the manuscript. All authors discussed the results and commented on the manuscript. Author Information Reprints and permissions information is available at www.nature.com/reprints. The authors declare no competing financial interests. Readers are welcome to comment on the online version of the paper. Correspondence and requests for materials should be addressed to J.P. ([email protected]
6 6 0 | N AT U R E | VO L 5 2 0 | 3 0 A P R I L 2 0 1 5 G2015
Macmillan Publishers Limited. All rights reserved